Ln2Ti2S2O5 (Ln = Nd, Pr, Sm): a novel series of defective Ruddlesden‒Popper phases
Goga, M.; Seshadri, R.; Ksenofontov, V.; Gütlich, P.; Tremel, W.; Chemical Communications  (1999) 979–; doi:10.1039/a809737b

data_7110441
_publ_section_title
;
 Ln2Ti2S2O5 (Ln = Nd, Pr, Sm): a novel series of defective
 Ruddlesden--Popper phases
;
_journal_issue                   11
_journal_name_full               'Chemical Communications'
_journal_page_first              979
_journal_paper_doi               10.1039/a809737b
_journal_year                    1999
_chemical_formula_sum            'Nd2 O5 S2 Ti2'
_chemical_formula_weight         528.40
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   3.8490(10)
_cell_length_b                   3.8490(10)
_cell_length_c                   23.064(5)
_cell_measurement_temperature    293(2)
_cell_volume                     341.69(15)
_computing_structure_refinement  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_solution    'SHELXS-86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0369
_diffrn_reflns_av_sigmaI/netI    0.0146
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_k_max       4
_diffrn_reflns_limit_k_min       -4
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            1728
_diffrn_reflns_theta_max         24.68
_diffrn_reflns_theta_min         1.77
_exptl_absorpt_coefficient_mu    17.763
_exptl_crystal_density_diffrn    5.136
_exptl_crystal_F_000             472
_refine_diff_density_max         1.020
_refine_diff_density_min         -1.125
_refine_diff_density_rms         0.195
_refine_ls_extinction_coef       0.0180(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_all   1.235
_refine_ls_goodness_of_fit_obs   1.235
_refine_ls_matrix_type           full
_refine_ls_number_parameters     17
_refine_ls_number_reflns         124
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.235
_refine_ls_restrained_S_obs      1.235
_refine_ls_R_factor_all          0.0168
_refine_ls_R_factor_obs          0.0168
_refine_ls_shift/esd_max         0.000
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0281P)^2^+0.8271P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.0415
_refine_ls_wR_factor_obs         0.0415
_reflns_number_observed          124
_reflns_number_total             124
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            809737bsup1.cif
_cod_data_source_block           okay2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.0281P)^2^+0.8271P] where P=(Fo^2^+2Fc^2^)/3' was
changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.0281P)^2^+0.8271P] where P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_database_code               7110441